#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:59:59 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179550 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/19/4501915.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4501915
loop_
_publ_author_name
'Parhi, Purnendu'
'Upreti, Shailesh'
'Ramanan, Arunachalam'
_publ_section_title
;
 Crystallization of Calcium Vanadate Solids from Solution: A Metathetic
 Route
;
_journal_issue                   12
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              5078
_journal_paper_doi               10.1021/cg100703h
_journal_volume                  10
_journal_year                    2010
_chemical_formula_moiety         '2(O3 V), 3(H2 O), 2(O), Ca'
_chemical_formula_sum            'Ca H6 O11 V2'
_chemical_formula_weight         324.01
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 102.439(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   16.952(4)
_cell_length_b                   6.9373(14)
_cell_length_c                   7.2921(15)
_cell_measurement_reflns_used    1956
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      25.03
_cell_measurement_theta_min      2.46
_cell_volume                     837.4(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.986
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0261
_diffrn_reflns_av_sigmaI/netI    0.0241
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            3854
_diffrn_reflns_theta_full        25.03
_diffrn_reflns_theta_max         25.03
_diffrn_reflns_theta_min         2.46
_exptl_absorpt_coefficient_mu    2.890
_exptl_absorpt_correction_T_max  0.829
_exptl_absorpt_correction_T_min  0.729
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    2.570
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             640
_exptl_crystal_size_max          0.210
_exptl_crystal_size_mid          0.097
_exptl_crystal_size_min          0.065
_refine_diff_density_max         1.095
_refine_diff_density_min         -1.413
_refine_diff_density_rms         0.222
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.205
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     89
_refine_ls_number_reflns         916
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.205
_refine_ls_R_factor_all          0.0763
_refine_ls_R_factor_gt           0.0732
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1008P)²+16.5511P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2006
_refine_ls_wR_factor_ref         0.2091
_reflns_number_gt                751
_reflns_number_total             804
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg100703h_si_001.cif
_cod_data_source_block           3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4501915
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
V1 V 0.07489(8) 0.0000 -0.0874(2) 0.0123(6) Uani 1 2 d S
V2 V 0.07388(8) 0.0000 0.41181(19) 0.0147(6) Uani 1 2 d S
Ca1 Ca 0.30452(15) 0.0000 0.0244(4) 0.0361(8) Uani 1 2 d S
O1 O 0.0441(5) 0.0000 0.1491(12) 0.0130(6) Uani 1 2 d S
O2 O 0.1297(5) 0.1892(13) 0.4425(13) 0.018(3) Uani 1 1 d .
O3 O 0.0441(5) 0.0000 0.6452(11) 0.021(4) Uani 1 2 d S
O4 O 0.1571(6) 0.1402(17) -0.0461(15) 0.029(2) Uani 0.50 1 d P
O5 O 0.2514(4) 0.2465(12) -0.2356(13) 0.084(3) Uani 1 1 d .
O6 O 0.4082(9) 0.0000 0.3174(16) 0.078(4) Uani 1 2 d S
O7 O 0.4153(8) 0.0000 -0.1486(19) 0.075(4) Uani 1 2 d S
O4D O 0.1035(7) 0.2150(15) -0.0721(16) 0.029(2) Uani 0.50 1 d P
O1W O 0.3054(7) 0.0000 0.5393(17) 0.071(3) Uani 1 2 d S
H1 H 0.2873 0.3176 -0.2781 0.04(3) Uiso 1 1 d R
H2 H 0.2210 0.1706 -0.3184 0.04(4) Uiso 1 1 d R
H3 H 0.3773 0.0399 -0.1818 0.04(4) Uiso 0.50 1 d PR
H4 H 0.4352 0.0577 -0.2300 0.04(3) Uiso 0.50 1 d PR
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4D V1 O4D 144.8(8) 6 .
O4D V1 O4 36.8(5) 6 6
O4D V1 O4 108.0(7) . 6
O4D V1 O4 108.0(7) 6 .
O4D V1 O4 36.8(5) . .
O4 V1 O4 71.1(8) 6 .
O4D V1 O1 94.4(4) 6 .
O4D V1 O1 94.4(4) . .
O4 V1 O1 102.5(4) 6 .
O4 V1 O1 102.5(4) . .
O4D V1 O3 94.9(4) 6 1_554
O4D V1 O3 94.9(4) . 1_554
O4 V1 O3 102.6(4) 6 1_554
O4 V1 O3 102.6(4) . 1_554
O1 V1 O3 149.0(4) . 1_554
O4D V1 O1 107.6(4) 6 5
O4D V1 O1 107.6(4) . 5
O4 V1 O1 144.4(4) 6 5
O4 V1 O1 144.4(4) . 5
O1 V1 O1 74.9(4) . 5
O3 V1 O1 74.0(4) 1_554 5
O4D V1 V2 104.2(4) 6 5
O4D V1 V2 104.2(4) . 5
O4 V1 V2 130.9(4) 6 5
O4 V1 V2 130.9(4) . 5
O1 V1 V2 111.0(3) . 5
O3 V1 V2 38.0(2) 1_554 5
O1 V1 V2 36.1(2) 5 5
O4D V1 V1 103.9(4) 6 5
O4D V1 V1 103.9(4) . 5
O4 V1 V1 130.9(4) 6 5
O4 V1 V1 130.9(4) . 5
O1 V1 V1 38.2(2) . 5
O3 V1 V1 110.8(2) 1_554 5
O1 V1 V1 36.7(2) 5 5
V2 V1 V1 72.81(6) 5 5
O2 V2 O2 109.7(7) 6 .
O2 V2 O1 99.4(4) 6 .
O2 V2 O1 99.4(4) . .
O2 V2 O3 98.0(4) 6 .
O2 V2 O3 98.0(4) . .
O1 V2 O3 149.5(4) . .
O2 V2 O3 125.1(3) 6 5_556
O2 V2 O3 125.1(3) . 5_556
O1 V2 O3 75.2(4) . 5_556
O3 V2 O3 74.3(4) . 5_556
O2 V2 V2 117.0(3) 6 5_556
O2 V2 V2 117.0(3) . 5_556
O1 V2 V2 111.5(3) . 5_556
O3 V2 V2 38.0(2) . 5_556
O3 V2 V2 36.3(2) 5_556 5_556
O2 V2 V1 118.0(3) 6 5
O2 V2 V1 118.0(3) . 5
O1 V2 V1 38.3(3) . 5
O3 V2 V1 111.3(2) . 5
O3 V2 V1 36.9(2) 5_556 5
V2 V2 V1 73.23(6) 5_556 5
O6 Ca1 O7 87.9(5) . .
O6 Ca1 O4D 64.5(3) . 7
O7 Ca1 O4D 63.4(3) . 7
O6 Ca1 O4D 64.5(3) . 4_545
O7 Ca1 O4D 63.4(3) . 4_545
O4D Ca1 O4D 104.8(5) 7 4_545
O6 Ca1 O5 135.5(2) . .
O7 Ca1 O5 78.9(3) . .
O4D Ca1 O5 71.6(3) 7 .
O4D Ca1 O5 137.7(3) 4_545 .
O6 Ca1 O5 135.5(2) . 6
O7 Ca1 O5 78.9(3) . 6
O4D Ca1 O5 137.7(3) 7 6
O4D Ca1 O5 71.6(3) 4_545 6
O5 Ca1 O5 83.5(4) . 6
O6 Ca1 O4 79.8(3) . 7
O7 Ca1 O4 79.8(3) . 7
O4D Ca1 O4 23.3(3) 7 7
O4D Ca1 O4 128.1(4) 4_545 7
O5 Ca1 O4 56.2(3) . 7
O5 Ca1 O4 137.3(3) 6 7
O6 Ca1 O4 79.8(3) . 4_545
O7 Ca1 O4 79.8(3) . 4_545
O4D Ca1 O4 128.1(4) 7 4_545
O4D Ca1 O4 23.3(3) 4_545 4_545
O5 Ca1 O4 137.3(3) . 4_545
O5 Ca1 O4 56.2(3) 6 4_545
O4 Ca1 O4 151.4(5) 7 4_545
O6 Ca1 O4 130.0(4) . .
O7 Ca1 O4 133.9(4) . .
O4D Ca1 O4 105.9(3) 7 .
O4D Ca1 O4 149.3(4) 4_545 .
O5 Ca1 O4 56.1(3) . .
O5 Ca1 O4 86.2(3) 6 .
O4 Ca1 O4 82.6(3) 7 .
O4 Ca1 O4 126.0(4) 4_545 .
O6 Ca1 O4 130.0(4) . 6
O7 Ca1 O4 133.9(4) . 6
O4D Ca1 O4 149.3(4) 7 6
O4D Ca1 O4 105.9(3) 4_545 6
O5 Ca1 O4 86.2(3) . 6
O5 Ca1 O4 56.1(3) 6 6
O4 Ca1 O4 126.0(4) 7 6
O4 Ca1 O4 82.6(3) 4_545 6
O4 Ca1 O4 43.4(5) . 6
O6 Ca1 O5 76.9(3) . 7
O7 Ca1 O5 134.64(19) . 7
O4D Ca1 O5 71.6(3) 7 7
O4D Ca1 O5 137.5(3) 4_545 7
O5 Ca1 O5 82.8(3) . 7
O5 Ca1 O5 139.48(15) 6 7
O4 Ca1 O5 55.8(3) 7 7
O4 Ca1 O5 136.6(3) 4_545 7
O4 Ca1 O5 54.7(3) . 7
O4 Ca1 O5 85.1(3) 6 7
O6 Ca1 O5 76.9(3) . 4_545
O7 Ca1 O5 134.64(19) . 4_545
O4D Ca1 O5 137.5(3) 7 4_545
O4D Ca1 O5 71.6(3) 4_545 4_545
O5 Ca1 O5 139.48(15) . 4_545
O5 Ca1 O5 82.8(3) 6 4_545
O4 Ca1 O5 136.6(3) 7 4_545
O4 Ca1 O5 55.8(3) 4_545 4_545
O4 Ca1 O5 85.1(3) . 4_545
O4 Ca1 O5 54.7(3) 6 4_545
O5 Ca1 O5 83.4(4) 7 4_545
O6 Ca1 H3 101.3 . .
O7 Ca1 H3 15.4 . .
O4D Ca1 H3 64.0 7 .
O4D Ca1 H3 76.4 4_545 .
O5 Ca1 H3 64.0 . .
O5 Ca1 H3 74.5 6 .
O4 Ca1 H3 75.2 7 .
O4 Ca1 H3 89.6 4_545 .
O4 Ca1 H3 118.6 . .
O4 Ca1 H3 125.0 6 .
O5 Ca1 H3 130.6 7 .
O5 Ca1 H3 145.2 4_545 .
V2 O1 V1 149.3(5) . .
V2 O1 V1 105.7(4) . 5
V1 O1 V1 105.1(4) . 5
V2 O3 V1 149.2(4) . 1_556
V2 O3 V2 105.7(4) . 5_556
V1 O3 V2 105.1(4) 1_556 5_556
V1 O4 Ca1 139.8(6) . 7
V1 O4 Ca1 122.7(6) . .
Ca1 O4 Ca1 97.4(3) 7 .
Ca1 O5 Ca1 97.2(3) . 7
Ca1 O5 H1 118.0 . .
Ca1 O5 H1 101.1 7 .
Ca1 O5 H2 99.7 . .
Ca1 O5 H2 124.6 7 .
H1 O5 H2 115.9 . .
Ca1 O7 H4 145.0 . .
Ca1 O7 H3 55.2 . .
H4 O7 H3 92.7 . .
V1 O4D Ca1 160.0(7) . 7
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
V1 O4D 1.565(10) 6
V1 O4D 1.565(10) .
V1 O4 1.672(10) 6
V1 O4 1.672(10) .
V1 O1 1.906(9) .
V1 O3 1.906(8) 1_554
V1 O1 1.970(8) 5
V1 V2 3.064(2) 5
V1 V1 3.077(3) 5
V2 O2 1.606(8) 6
V2 O2 1.606(8) .
V2 O1 1.873(9) .
V2 O3 1.877(8) .
V2 O3 1.953(8) 5_556
V2 V2 3.052(3) 5_556
V2 V1 3.064(2) 5
Ca1 O6 2.458(12) .
Ca1 O7 2.478(12) .
Ca1 O4D 2.496(10) 7
Ca1 O4D 2.496(10) 4_545
Ca1 O5 2.568(9) .
Ca1 O5 2.568(9) 6
Ca1 O4 2.576(11) 7
Ca1 O4 2.576(11) 4_545
Ca1 O4 2.628(12) .
Ca1 O4 2.628(12) 6
Ca1 O5 2.644(9) 7
Ca1 O5 2.644(9) 4_545
Ca1 H3 2.1581 .
O1 V1 1.970(8) 5
O3 V1 1.906(8) 1_556
O3 V2 1.953(8) 5_556
O4 Ca1 2.576(11) 7
O5 Ca1 2.644(9) 7
O5 H1 0.8892 .
O5 H2 0.8792 .
O7 H4 0.8438 .
O7 H3 0.6957 .
O4D Ca1 2.496(10) 7
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O2 V2 O1 V1 -56.0(3) 6 .
O2 V2 O1 V1 56.0(3) . .
O3 V2 O1 V1 180.0 . .
O3 V2 O1 V1 180.0 5_556 .
V2 V2 O1 V1 180.0 5_556 .
V1 V2 O1 V1 180.000(1) 5 .
O2 V2 O1 V1 124.0(3) 6 5
O2 V2 O1 V1 -124.0(3) . 5
O3 V2 O1 V1 0.0 . 5
O3 V2 O1 V1 0.0 5_556 5
V2 V2 O1 V1 0.0 5_556 5
O4D V1 O1 V2 72.9(4) 6 .
O4D V1 O1 V2 -72.9(4) . .
O4 V1 O1 V2 36.6(4) 6 .
O4 V1 O1 V2 -36.6(4) . .
O3 V1 O1 V2 180.0 1_554 .
O1 V1 O1 V2 180.0 5 .
V2 V1 O1 V2 180.0 5 .
V1 V1 O1 V2 180.0 5 .
O4D V1 O1 V1 -107.1(4) 6 5
O4D V1 O1 V1 107.1(4) . 5
O4 V1 O1 V1 -143.4(4) 6 5
O4 V1 O1 V1 143.4(4) . 5
O3 V1 O1 V1 0.0 1_554 5
O1 V1 O1 V1 0.0 5 5
V2 V1 O1 V1 0.0 5 5
O2 V2 O3 V1 55.7(3) 6 1_556
O2 V2 O3 V1 -55.6(3) . 1_556
O1 V2 O3 V1 180.0 . 1_556
O3 V2 O3 V1 180.000(1) 5_556 1_556
V2 V2 O3 V1 180.000(2) 5_556 1_556
V1 V2 O3 V1 180.0 5 1_556
O2 V2 O3 V2 -124.3(3) 6 5_556
O2 V2 O3 V2 124.4(3) . 5_556
O1 V2 O3 V2 0.000(2) . 5_556
O3 V2 O3 V2 0.0 5_556 5_556
V1 V2 O3 V2 0.0 5 5_556
O4D V1 O4 Ca1 -179.1(8) 6 7
O4D V1 O4 Ca1 0.2(8) . 7
O4 V1 O4 Ca1 -179.4(6) 6 7
O1 V1 O4 Ca1 -80.3(9) . 7
O3 V1 O4 Ca1 81.4(9) 1_554 7
O1 V1 O4 Ca1 1.3(14) 5 7
V2 V1 O4 Ca1 52.4(11) 5 7
V1 V1 O4 Ca1 -51.1(11) 5 7
O4D V1 O4 Ca1 1.0(8) 6 .
O4D V1 O4 Ca1 -179.8(12) . .
O4 V1 O4 Ca1 0.7(8) 6 .
O1 V1 O4 Ca1 99.8(5) . .
O3 V1 O4 Ca1 -98.5(6) 1_554 .
O1 V1 O4 Ca1 -178.7(4) 5 .
V2 V1 O4 Ca1 -127.5(5) 5 .
V1 V1 O4 Ca1 129.0(4) 5 .
O6 Ca1 O4 V1 -110.1(6) . .
O7 Ca1 O4 V1 112.0(6) . .
O4D Ca1 O4 V1 -180.0(6) 7 .
O4D Ca1 O4 V1 -1.8(11) 4_545 .
O5 Ca1 O4 V1 126.0(7) . .
O5 Ca1 O4 V1 41.3(6) 6 .
O4 Ca1 O4 V1 180.0(9) 7 .
O4 Ca1 O4 V1 -1.3(5) 4_545 .
O4 Ca1 O4 V1 -0.6(7) 6 .
O5 Ca1 O4 V1 -127.1(8) 7 .
O5 Ca1 O4 V1 -41.8(6) 4_545 .
O6 Ca1 O4 Ca1 69.9(5) . 7
O7 Ca1 O4 Ca1 -68.0(5) . 7
O4D Ca1 O4 Ca1 0.1(4) 7 7
O4D Ca1 O4 Ca1 178.2(6) 4_545 7
O5 Ca1 O4 Ca1 -54.0(3) . 7
O5 Ca1 O4 Ca1 -138.7(4) 6 7
O4 Ca1 O4 Ca1 0.0 7 7
O4 Ca1 O4 Ca1 178.8(4) 4_545 7
O4 Ca1 O4 Ca1 179.4(2) 6 7
O5 Ca1 O4 Ca1 52.9(3) 7 7
O5 Ca1 O4 Ca1 138.3(4) 4_545 7
O6 Ca1 O5 Ca1 -62.9(5) . 7
O7 Ca1 O5 Ca1 -138.3(3) . 7
O4D Ca1 O5 Ca1 -72.9(3) 7 7
O4D Ca1 O5 Ca1 -164.9(4) 4_545 7
O5 Ca1 O5 Ca1 141.77(16) 6 7
O4 Ca1 O5 Ca1 -53.3(3) 7 7
O4 Ca1 O5 Ca1 160.3(4) 4_545 7
O4 Ca1 O5 Ca1 51.9(3) . 7
O4 Ca1 O5 Ca1 85.5(3) 6 7
O5 Ca1 O5 Ca1 0.0 7 7
O5 Ca1 O5 Ca1 70.9(5) 4_545 7
O4D V1 O4D Ca1 1(3) 6 7
O4 V1 O4D Ca1 0(2) 6 7
O4 V1 O4D Ca1 -0.3(15) . 7
O1 V1 O4D Ca1 104.8(19) . 7
O3 V1 O4D Ca1 -104.9(19) 1_554 7
O1 V1 O4D Ca1 -179.7(18) 5 7
V2 V1 O4D Ca1 -142.3(18) 5 7
V1 V1 O4D Ca1 142.3(18) 5 7
